**To link to this article: **

### DOI:10.1103/PhysRevLett.91.247001

### http://dx.doi.org/10.1103/PhysRevLett.91.247001

### This is a

### n author-deposited version published in:

### http://oatao.univ-toulouse.fr/

### Eprints ID: 5282

**To cite this version: **

### Connétable, Damien and Timoshevskii, V. and Masenelli, B. and Beille, J. and

### Marcus, J. and Barbara, B. and Saitta, A.M. and Rignanese, G.M. and M

### élinon,

*P. and Yamanaka, S. and Blase, X. Superconductivity in doped sp3 *

*semiconductors: The case of the clathrates. (2003) Physicla Review Letters, vol. *

### 91 (n° 24). pp. 247001-247001.

## O

## pen

## A

## rchive

## T

## oulouse

## A

## rchive

## O

## uverte (

## OATAO

## )

### OATAO is an open access repository that collects the work of Toulouse researchers and

### makes it freely available over the web where possible.

### Any correspondence concerning this service should be sent to the repository

### administrator:

### staff-oatao@inp-toulouse.fr

**Superconductivity in Doped sp**

**Superconductivity in Doped sp**

**3**

_{Semiconductors: The Case of the Clathrates}

_{Semiconductors: The Case of the Clathrates}

D. Conne´table,1V. Timoshevskii,1B. Masenelli,1J. Beille,3J. Marcus,4B. Barbara,3A. M. Saitta,2G.-M. Rignanese,5 P. Me´linon,1S. Yamanaka,6and X. Blase1

1_{LPMCN, Universite´ Claude Bernard Lyon I and CNRS, UMR 5586, Baˆtiment Brillouin, 43 Bd du 11 Novembre 1918,}

*69622 Villeurbanne Cedex, France*

2_{LPMC, Universite´ Pierre et Marie Curie (Paris 6) and CNRS, UMR 7602, Tour 13/14, 4 Place Jussieu,}

*75252 Paris Cedex 05, France*

3* _{Laboratoire Louis Ne´el, CNRS, BP 166, 38042, Grenoble, France}*
4

_{LEPES, CNRS, BP 166, 38042, Grenoble, France}5_{Universite´ Catholique de Louvain, Unite´ de Physico-Chimie et de Physique des Mate´riaux,}

*1 Place Croix du Sud, B-1348 Louvain-la-Neuve, Belgium*

6_{Department of Applied Chemistry, Faculty of Engineering, Hiroshima University,}

*1-4-1 Kagamiyama, Higashi-Hiroshima, Hiroshima 739-8527, Japan*

We present a joint experimental and theoretical study of the superconductivity in doped silicon clathrates. The critical temperature in Ba8@Si-46 is shown to strongly decrease with applied pressure.

*These results are corroborated by ab initio calculations using MacMillan’s formulation of the BCS*
*theory with the electron-phonon coupling constant calculated from perturbative density functional*
theory. Further, the study of I8@Si-46 and of gedanken pure silicon diamond and clathrate phases doped

*within a rigid-band approach show that the superconductivity is an intrinsic property of the sp*3_{silicon}

network. As a consequence, carbon clathrates are predicted to yield large critical temperatures with an effective electron-phonon interaction much larger than in C60.

DOI: 10.1103/PhysRevLett.91.247001

The superconductivity in column-IV elemental
com-pounds has been extensively studied in the case of carbon.
*In particular, the large observed critical temperature (Tc*)

in doped C_{60} fullerene networks has stimulated a lot of
work [1] while recent theoretical predictions emphasized
that by reducing the fullerene size down to C_{36}[2] or even
C28 *[3], Tc* could be significantly increased.

*Contrary to carbon, silicon does not form sp*2_{-like}

networks and, at ambient pressure, there is no
*supercon-ductivity associated with the sp*3 _{diamond phase. It is}

only at higher pressure, upon phase transformation into
*metallic phases such as the -tin and simple hexagonal*
(sh-V) phases at 11 and 13–14 GPa, respectively, that
*superconductivity with a Tc* of 6 –8 K could be measured

and explained using electron-phonon calculations within the BCS theory [4].

The absence of superconductivity in silicon or carbon
*sp*3 _{networks raises the problem of the doping of such}

dense insulating phases. High doping changes the average
lattice constant and introduces mechanical stresses with
misfit dislocations [5]. In addition, doping is always
limited by the solubility limit for the impurity in the
solid which is small at low temperature. Practically, in
*heavily n-doped silicon, the well known ‘‘doping rule*
limit’’ predicts [6] a Fermi level located a few tenths of
eVabove the conduction band minimum (CBM) where the
electronic density of states (EDOS) is not large enough to
induce superconductivity.

In this perspective, silicon clathrates [7] are promising candidates as they are cagelike materials allowing

inter-calation. In the case of the type-I clathrates studied here,
they are built from a regular arrangement of a
combina-tion of Si20*(Ih*) and Si24*(D6d*) cages (Fig. 1). Contrary to

C60 fullerene-assembled films, the silicon cages are

strongly linked together since the polyhedra share
pen-tagonal and hexagonal faces. All silicon atoms are thus
*covalently bonded within a four-neighbor sp*3 _{}

environ-ment as in the diamond phase, and silicon clathrates are
*1:8 eV band gap semiconductors [8]. Doping of type-I*
*clathrates leads to a X*_{8}*@Si-46 stoichiometry, where X is*
*the in-cage guest atom, displaying thus a huge 8=46 ratio*
of intercalated to host network atoms. As a result, the
*Fermi level (Ef*) can be strongly displaced in the valence

or conduction bands.

FIG. 1. Symbolic representation of face sharing Si20and Si24

*In the case of barium intercalation [9 –13], E _{f}* is
lo-cated around 1 eV above the CBM near a peak in the

*EDOS related to a hybridization between the Ba-5d*orbi-tals and the Si antibonding states [14]. This has been invoked to be at the origin of the 8 K superconductivity in Ba8@Si-46 as reported originally in Ref. [9]. Besides

the superconducting properties, these novel phases have recently attracted much attention for the evolution under doping of their pressure-related phase diagram [15], ther-moelectric power [16], or band gap [17].

In this Letter, we report on a joint experimental and
theoretical study of the superconductivity in doped
sili-con clathrates. Experimentally, in the case of Ba_{8}@Si-46,
*the pressure is found to strongly reduce T _{c}*. These results
are reproduced within the BCS theory where the

*electron-phonon coupling constant is calculated ab initio from*density functional perturbative theory (DFPT) [18]. To understand the origin of the superconductivity in such

*compounds, the cases of p-doped I*

_{8}@46 and empty Si-46 clathrates ‘‘artificially doped’’ within a rigid-band approach are studied on the same theoretical footing. Our results show that the superconductivity is an intrinsic

*property of the sp*3

_{silicon network. Further, we predict}

that the synthesis of carbon clathrates would lead to
*relatively high Tc* compounds.

Ba8@Si-46 samples were prepared following Ref. [19].

Starting from the BaSi_{2} Zintl phase mixed with silicon
*powder and placed in an h-BN cell, the synthesis occurs at*
1000 K under high pressure (1–5 GPa). The sample is
quenched at room temperature before the pressure is
slowly released. The electrical resistivity was measured
using a four-wires–type method. Wires were glued with
silver varnish and electrical contact improved by
anneal-ing. Hydrostatic pressure, up to 18 kbar, was generated in
a beryllium-copper self-clamped vessel, in which the
samples were pressurized inside a Teflon capsule by a
*50=50 pentane-isoamyl alcohol mixture. Pressure was*
applied at room temperature and the resistivity curves
were recorded upon cooling. The reproducibility of the
data was checked for each set of measurements,
indicat-ing that the sample did not degrade upon pressure or
thermal cycling. The superconducting transition
*tempera-ture T _{c}*is determined at the maximum of the derivative of

*resistivity versus temperature. As shown in Fig. 2, T*decreases with pressure. Another doped clathrate labeled Ba

_{c}_{8}@Si-40Ag-6 was prepared by substituting some of the silicon atoms by silver. This sample is metalliclike with-out superconductivity down to 1.5 K.

Our calculations are performed within the local
den-sity approximation to the denden-sity functional theory [20]
and a pseudopotential [21] plane-wave approach. A 16 Ryd
energy cutoff and a 2 2 2 Monkhorst-Pack [22]
sam-pling of the Brillouin zone showed good convergency for
structural relaxations. The electron-phonon coupling
*ma-trix elements [23], h *0

* nkj ^q V=Rj *0

*i, were*

**nkq**ob-tained within the framework of DFPT [18]. Because of

the computational cost, phonons were calculated at the

**q **point only. We recall that the unit cell contains 46
silicon and 8 dopants atoms. In particular, two Si_{20}cages
are present. Therefore, not only on-ball but also interball
phonons are considered within our sampling. Together
with the choice of the screened electron-electron
*inter-action * *which enters the evaluation of T _{c}* (see below)

**and the use of the MacMillan formula, this q-point**sam-pling certainly limits the accuracy of the present calcu-lations. We will comment upon this point when comparing our results with the experimental one.

For the calculation of the variation of the total
**poten-tial V=R and of ,**

* NEfVep 2NEf*

X

*hhjgq*j2*ii= h!q;*

*where hhjg q*j2

*0 average electron-phonon coupling matrix elements for states over the*

**ii is related to the k; k****Fermi surface [23], a larger 8 8 8 k-point sampling**

*was used. The quantity Vep* represents an average

electron-phonon interaction strength per electronic state
*at E _{f}*

*[with NE*

_{f}**in states=eV]. The knowledge of***allows one to compute T*following Mac Millan [24]:

_{c}*Tc*
*h!*log
*1:2k _{B}*exp

_{ 1:041 }

*1 0:62*

*;*

*where !*

_{log}expP

*qlog!qq=*

P

*qq*. The value

*of *, which is the effective electron-electron repulsive
interaction, is certainly one of the main problems in the
*calculation of Tc. In the present work, we adjust * to the

*value needed to reproduce the Tc* 8 K of Ba8@Si-46 at

ambient pressure. For calculations at higher pressure and
*for different doping (see below), *is kept to be the same
*[25]. What we seek to reproduce is therefore the evolution*
*of T _{c}* either as a function of pressure or as a function

*of doping. Our fitted value is*

*0:24. This can be*

FIG. 2. (a) Evolution of the resistivity (normalized by its value at 300 K) of Ba8@Si-46 as a function of temperature

*for different pressures. (b) Evolution of Tc*under pressure as a
*function of the a=a*0*lattice parameter ratio (a*0 ambient

pres-sure lattice parameter). The open circles represent the experi-mental data and the solid squares the theoretical values. The dashed line is a guide to the eyes.

*compared to the values of 0:1–0:2 for good elemental*
*metals and to 0:1–0:3 for C*_{60}, C_{36}, and C_{28}.

We compare in Fig. 2 the theoretical and experimental
*variations of T _{c}* in Ba

_{8}@Si-46 upon pressure. The excel-lent agreement between theory and experiment concern-ing this evolution is a solid indication that the BCS theory and our computational framework is able to capture the main physics of such systems. The experimental slope

*dT=da 17:1 K*A 1 is, indeed, close to the theoretical

*18:7 K*A 1

*. We report in Table I the evolution of under*

*pressure. The EDOS at the Fermi level, NEf, and Vep*

are found to decrease by 30% and 20%, respectively,
*contributing both to the collapse of T _{c}*.

We now try to understand the origin of
superconduc-tivity in Ba_{8}@Si-46. We represent in Fig. 3 the phonon
band structure, density of states (pDOS), and coupling
*constant ! related to phonons with energy ! only.*
Contrary to the case of fullerides, where specific
on-ball phonon modes were found to be responsible for
super-conductivity, it is difficult to extract specific phonon and
*electronic modes with dominant participation to .*

*To gain further insight, we calculate Tcfor the p-doped*

I8*@Si-46 clathrate [17,26]. As shown in Table I, Vep*and

*Tc* are very similar to the ones obtained with Ba doping.

These results show that superconductivity in doped
*clath-rates is not specifically related to Ba and to the d *
charac-ter of its oucharac-ter electrons. In the case of Na-doped
*clathrates, V _{ep}* is actually larger than in the case of

*Ba-doped clathrate, and it is the collapse of NE*which

_{f}*reduces T _{c}*to very small values, in good agreement with
experiment.

In both I and Ba cases, hybridization between Si and
intercalated atoms may be interpreted as leading to a
coordination which is larger than 4, thus making doped
Si clathrates highly coordinated phases equivalent to
high-pressure superconducting phases of silicon. To
*ex-plore this hypothesis, we further calculate Tc* for empty

clathrates doped within a rigid-band model. Namely,
**using the V=R matrix elements and electronic states***calculated for the empty Si-46 phase, the values of ,*
*NEf, and Tc* *were calculated by locating artificially Ef*

above or below the band gap, thus allowing the phonons
to couple with electronic states at different energies. The
*results are given in Table I. Again, we find that V _{ep}* is
rather stable, with values comparable to the one of
Ba-or I-doped clathrates, and that the superconductivity is

*mainly related to NE*.

_{f}Further, we have performed the same rigid-band
analy-sis in the silicon diamond phase [27]. The coupling
*con-stant is found to range between 0.4 – 0.7 for Ef*located

*up to 1 eV above the CBM. With a !*log 450 K prefactor,

*and with * * 0:24, the critical temperature is found to*
be in the {0 –5 K} energy range, which compares
reason-ably well with the clathrate case where we could not find
any ‘‘cage-related’’ modes contributing preferentially to
*. These results show that sp*3_{silicon networks in general}

lead intrinsically to a large electron-phonon coupling and
*that T _{c}* of 8 K can be obtained provided that sufficient
doping is available. These findings are consistent with the

*collapse of T*in Ba

_{c}_{8}@Si-40Ag-6 compounds where the silver noble metal in substitution in the Si network

*de-stroys its sp*3

_{character.}

We now conclude our study by exploring the case of the hypothetical carbon clathrates. As such phases are com-posed of C20and C24cages, it is tempting to extrapolate

the results obtained for free C60, C36, and C28 clusters

*[2,3] which predict an increase of Tc* with decreasing

sphere radius. However, as in the clathrate phase the cages
are sharing faces, such an extrapolation is subject to
caution. Nevertheless, the present results suggest that
*superconductivity can occur in doped sp*3 _{column-IV}

FIG. 3. Phonon band structure, the pDOS of Ba8@Si-46 at

*ambient pressure and the coupling constant !.*
TABLE I. *, NEf (states=eV), !*log*(K), Vep(meV), and Tc*

(K) as a function of (left column) the reduced lattice parameter
*a=a*0 for Ba8@Si-46, different doping elements, and various

*positions of Ef* *on the rigid-band model (see text). Ef* is given
with respect to the top of the valence bands (bottom of the
conduction bands) when negative (positive).

*a=a*0 *NEf (Ef*) *Vep* *h!*logi *Tc*
1.0 1.05 43 (0.9) 24 280 8.4
0.992 0.96 41 23 290 6.9
0.984 0.87 39.5 22 300 4.9
0.969 0.76 37.5 20 314 2.7
0.938 0.58 30 19 326 0.4
Element M
Na 0.40 15.3 (0.7) 26 360 1
I 0.90 *44.4 (
0:26)* 20 300 5.9
*Ef* *NEf* *Vep* *h!*logi (K) *Tc*(K)
*
0:6* 1.00 51 19 432 11
*
0:4* 0.77 23 33 466 4.6
*0:3* 0.20 7.4 27 600 0
*0:5* 0.41 17.6 23 470 0
*0:7* 0.55 20.5 26 405 0.3
*0:9* 0.61 26.4 23 366 0.6

materials. Following the rigid-band scheme adopted for
silicon clathrates, and with an average phonon frequency
*!*_{log}* 1500 K, our ab initio evaluation of yields values*
*as large as 1.4 for E _{f}* located up to 1 eV above the CBM.

*Our values for V*range between 150 –250 meV which

_{ep}*can be compared to the 210 meV found by Breda et al. for*isolated C28 clusters [3]. It is, in particular, much larger

than the 60 meV value found for C60[1], suggesting that

*purely sp*3_{network can be even more efficient in yielding}

*superconductivity than the ‘‘curved sp*2_{systems’’ }

consid-ered so far [28].

In conclusion, we have presented a combined
experi-mental and theoretical study of the superconductivity in
doped silicon clathrates. The critical temperature of
Ba_{8}@Si-46 and its decrease under pressure is well
repro-duced within the BCS theory with electron-phonon
*cou-pling constants calculated ab initio. Our results show that*
superconductivity in doped silicon clathrates is an
*intrin-sic property of the sp*3 _{network and is not specifically}

*related to the Ba-5d states or an increase of coordination*
under doping. As a result, we show that large critical
temperatures can be expected for the hypothetical carbon
clathrate phases. As shown in Ref. [29], an efficient
doping of carbon clathrates could be obtained by Li
intercalation or boron substitution.

Calculations have been performed at the French CNRS national computer center at IDRIS (Orsay). X. B. is indebted to P. Quemerais and M. Coˆte´ for stimulating discussions.

*Note added.—In two recent papers published after *
*sub-mission of our manuscript, our calculated values for and*
in Ba_{8}@Si-46 were confirmed experimentally [30],
*and similar results concerning the prediction of T _{c}* in
doped carbon clathrates were obtained [31].

**[1] O. Gunnarsson, Rev. Mod. Phys. 69, 575 (1997).**
[2] M. Coˆte´, J. C. Grossman, M. L. Cohen, and S. G. Louie,

**Phys. Rev. Lett. 81, 697 (1998).**

**[3] N. Breda et al., Phys. Rev. B 62, 130 (2000).****[4] K. J. Chang et al., Phys. Rev. Lett. 54, 2375 (1985).****[5] D. J. Chadi et al., Phys. Rev. Lett. 79, 4834 (1997); P. H.**

**Citrin et al., Phys. Rev. Lett. 83, 3234 (1999).**

[6] S. B. Zhang, S.-H. Wei, and A. Zunger, Phys. Rev. Lett.

**84, 1232 (2000).**

**[7] J. S. Kasper et al., Science 150, 1713 (1965).**

**[8] E. Galvani et al., Phys. Rev. Lett. 77, 3573 (1996); J.****Gryco et al., Phys. Rev. B 62, R7707 (2000); X. Blase,****Phys. Rev. B 67, 035211 (2003).**

[9] H. Kawaji, H.-O. Horie, S. Yamanaka, and M. Ishikawa,
**Phys. Rev. Lett. 74, 1427 (1995).**

* [10] H. Sakamoto et al., Physica (Amsterdam) 341C, 2135*
(2000).

[11] S. Yamanaka, H. O. Horie, H. Kawaji, and M. Ishikawa,
**Eur. J. Solid State Inorg. Chem. 32, 799 (1995).**

* [12] I. M. Gat et al., Physica (Amsterdam) 289B, 385*
(2000).

[13] Y. Nozue, G. Hosaka, E. Enishi, and S. Yamanaka,
**Mol. Cryst. Liq. Cryst. 341, 509 (2000); H. Fukuoka,**
**J. Kiyoto, and S. Yamanaka, Inorg. Chem. 42, 2933**
(2003).

**[14] S. Saito and A. Oshiyama, Phys. Rev. B 51, 2628 (1995);**
**T. Yokoya et al., Phys. Rev. B 64, 172504 (2001).****[15] A. San Miguel et al., Phys. Rev. Lett. 83, 5290 (1999);**

**Phys. Rev. B 65, 054109 (2002); J. S. Tse et al., Phys.****Rev. Lett. 89, 195507 (2002); T. Kume et al., Phys. Rev.****Lett. 90, 155503 (2003).**

**[16] J. L. Cohn et al., Phys. Rev. Lett. 82, 779 (1999); J. S. Tse****et al., Phys. Rev. Lett. 85, 114 (2000).**

[17] D. Conne´table, V. Timoshevskii, E. Artacho, and X.
**Blase, Phys. Rev. Lett. 87, 206405 (2001).**

[18] S. Baroni, S. de Gironcoli, A. Dal Coso, and P.
**Giannozzi, Rev. Mod. Phys. 73, 515 (2001); S. Baroni,**
A. Dal Corso, S. de Gironcoli, and P. Giannozzi, http://
www.pwscf.org.

[19] S. Yamanaka, E. Enishi, H. Fukuoka, and M. Yasukawa,
**Inorg. Chem. 39, 56 (2000).**

**[20] P. Hohenberg and W. Kohn, Phys. Rev. 136, B864 (1964);**
**D. M. Ceperley and B. J. Alder, Phys. Rev. Lett. 45,**
566 (1980).

**[21] N. Troullier and J. L. Martins, Phys. Rev. B 43, 1993**
(1991); L. Kleinman and D. M. Bylander, Phys. Rev.
**Lett. 48, 1425 (1982).**

**[22] H. J. Monkhorst and J. D. Pack, Phys. Rev. B 13, 5188**
(1976).

[23] We follow the notations of M. M. Dacarogna and M. L.
**Cohen, Phys. Rev. Lett. 55, 837 (1985).**

**[24] W. L. McMillan, Phys. Rev. 167, 331 (1968).**

[25] An empirical relation for the variation under pressure of
*with NEF* is provided in M. M. Dacarogna, M. L.
**Cohen, and P. K. Lam, Phys. Rev. B 34, 4865 (1986).**
*With this relation, * _{does not change by more that 1%}

*between our two extreme values for NEF*.
**[26] E. Re´ny et al., Phys. Rev. B 66, 014532 (2002).**

**[27] The k- and q-point samplings were increased, **
respec-tively, to 30 30 30 and 6 6 6 grids.

*[28] For free carbon clusters, the increase in sp*3 _{character}

with decreasing radius has been often invoked to explain
*the upward evolution of Vep*. Our study confirms that
*maximizing the sp*3 _{character of the carbon network}

increases the electron-phonon coupling.

[29] M. Bernasconi, S. Gaito, and G. Benedek, Phys. Rev. B

**61, 12 689 (2000).**

**[30] K. Tanigaki et al., Nature Mater. 2, 653 (2003).**

[31] I. Spagnolatti, M. Bernasconi, and G. Benedek, Eur.
**Phys. J. B 34, 63 (2003).**